- Nano Express
- Open Access
Annealing effect on Sb2S3-TiO2 nanostructures for solar cell applications
Nanoscale Research Letters volume 8, Article number: 89 (2013)
Nanostructures composited of vertical rutile TiO2 nanorod arrays and Sb2S3 nanoparticles were prepared on an F:SnO2 conductive glass by hydrothermal method and successive ionic layer adsorption and reaction method at low temperature. Sb2S3-sensitized TiO2 nanorod solar cells were assembled using the Sb2S3-TiO2 nanostructure as the photoanode and a polysulfide solution as an electrolyte. Annealing effects on the optical and photovoltaic properties of Sb2S3-TiO2 nanostructure were studied systematically. As the annealing temperatures increased, a regular red shift of the bandgap of Sb2S3 nanoparticles was observed, where the bandgap decreased from 2.25 to 1.73 eV. At the same time, the photovoltaic conversion efficiency for the nanostructured solar cells increased from 0.46% up to 1.47% as a consequence of the annealing effect. This improvement can be explained by considering the changes in the morphology, the crystalline quality, and the optical properties caused by the annealing treatment.
Dye-sensitized solar cells (DSSCs) pioneered by O'Regan and Grätzel have been intensively investigated as a promising photovoltaic cell all over the world [1–5]. Until now, photovoltaic conversion efficiency of up to 11% has been reported for DSSCs in the laboratory . Although the conversion efficiency is impressive, the expense of the dye required to sensitize the solar cell is still not feasible for practical applications. Therefore, it is critical to tailor the materials to be not only cost effective but also long lasting. Recently, the utilization of narrow-bandgap semiconductors as a light-absorbing material, in place of conventional dye molecules, has drawn much attention. Inorganic semiconductors have several advantages over conventional dyes: (1) The bandgap of semiconductor nanoparticles can be easily tuned by size over a wide range to match the solar spectrum. (2) Their large intrinsic dipole moments can lead to rapid charge separation and large extinction coefficient, which is known to reduce the dark current and increase the overall efficiency. (3) In addition, semiconductor sensitizers provide new chances to utilize hot electrons to generate multiple charge carriers with a single photon. These properties make such inorganic narrow-bandgap semiconductors extremely attractive as materials for photovoltaic applications.
Recently, a range of nano-sized semiconductors has been investigated in photovoltaic applications including CdS [7–9], CdSe [10–13], Ag2S , In2S3, PbS , Sb2S3, Cu2O , as well as III-VI quantum ring . Among these narrow-bandgap semiconductors, Sb2S3 has shown much promise as an impressive sensitizer due to its reasonable bandgap of about 1.7 eV, exhibiting a strong absorption of the solar spectrum. The use of Sb2S3 nanoparticles, which may produce more than one electron–hole pair per single absorbed photon (also known as multiple exciton generation), is a promising solution to enhance power conversion efficiency. Furthermore, the creation of a type-II heterojunction by growing Sb2S3 nanoparticles on the TiO2 surface greatly enhances charge separation. All of these effects are known to increase the exciton concentration, lifetime of hot electrons, and therefore, the performance of sensitized solar cells. Limited research has previously been carried out with Sb2S3-TiO2 nanostructure for solar cell applications [20–22]. A remarkable performance was obtained in both liquid cell configuration and solid configuration. These findings were based on the use of porous nanocrystalline TiO2 particles; however, very little research has been conducted using single-crystalline TiO2 nanorod arrays. Compared with conventional porous polycrystalline TiO2 films, single-crystalline TiO2 nanorods grown directly on transparent conductive oxide electrodes provide an ideal alternative solution by avoiding particle-to-particle hopping that occurs in polycrystalline films, thereby increasing the photocurrent efficiency. Further enhancements in solid Sb2S3-sensitized solar cells demand a deeper understanding of the main parameters determining photoelectric behavior while also requiring additional research and insight into the electrical transporting process in these nanostructures.
In our present research study, Sb2S3 semiconductor nanoparticles and single-crystalline rutile TiO2 nanorod arrays were combined to perform as a photoanode for a practical nanostructured solar cell (as depicted in Figure 1). The annealing effect on the photovoltaic performance and optical property of Sb2S3-TiO2 nanostructures was studied systematically, and the optimal temperature of 300°C was confirmed. After annealing, apparent changes of morphological, optical, and photovoltaic properties were observed. The photovoltaic conversion efficiency of solar cell assembled using annealed Sb2S3-TiO2 nanostructure demonstrated a significant increase of 219%, compared with that based on as-made Sb2S3-TiO2 nanostructure.
Growth of single-crystalline rutile TiO2 nanorod arrays by hydrothermal process
TiO2 nanorod arrays were grown directly on fluorine-doped tin oxide (FTO)-coated glass using the following hydrothermal methods: 50 mL of deionized water was mixed with 40 mL of concentrated hydrochloric acid. After stirring at ambient temperature for 5 min, 400 μL of titanium tetrachloride was added to the mixture. The feedstock, prepared as previously described, was injected into a stainless steel autoclave with a Teflon lining. The FTO substrates were ultrasonically cleaned for 10 min in a mixed solution of deionized water, acetone, and 2-propanol with volume ratios of 1:1:1 and were placed at an angle against the Teflon liner wall with the conducting side facing down. The hydrothermal synthesis was performed by placing the autoclave in an oven and keeping it at 180°C for 2 h. After synthesis, the autoclave was cooled to room temperature under flowing water, and the FTO substrates were taken out, washed extensively with deionized water, and dried in open air.
Deposition of Sb2S3 nanoparticles with successive ionic layer adsorption and reaction method and annealing treatment
Successive ionic layer adsorption and reaction (SILAR) method was used to prepare Sb2S3 semiconductor nanoparticles. In a typical SILAR cycle, the F:SnO2 conductive glass, pre-grown with TiO2 nanorod arrays, was dipped into the 0.1 M antimonic chloride ethanol solution for 5 min at 50°C. Next, the F:SnO2 conductive glass was rinsed with ethanol and then dipped in 0.2 M sodium thiosulfate solution for 5 min at 80°C and finally rinsed in water. This entire SILAR process was repeated for 10 cycles. After the SILAR process, samples were annealed in N2 flow at varied temperatures from 100°C to 400°C for 30 min. After annealing, a color change was noted in the Sb2S3-TiO2 nanostructured samples, which were orange before annealing and gradually turned blackish as the annealing temperature increased.
Characterization of the Sb2S3-TiO2 nanostructures
The crystal structure of the Sb2S3-TiO2 samples were examined by X-ray diffraction (XD-3, PG Instruments Ltd., Beijing, China) with CuKα radiation (λ = 0.154 nm) at a scan rate of 2°/min. X-ray tube voltage and current were set at 40 kV and 30 mA, respectively. The surface morphology of the Sb2S3-TiO2 nanostructures was examined by scanning electron microscopy (SEM; FEI Sirion, FEI Company, Hillsboro, OR, USA). The optical absorption spectra were obtained using a dual beam UV-visible spectrometer (TU-1900, PG Instruments, Ltd.).
Solar cell assembly and performance measurement
Solar cells were assembled using a Sb2S3-TiO2 nanostructure as the photoanode. Pt counter electrodes were prepared by depositing an approximately 20-nm Pt film on FTO glass using magnetron sputtering. A 60-μm-thick sealing material (SX-1170-60, Solaronix SA, Aubonne, Switzerland) with a 3 × 3 mm aperture was pasted onto the Pt counter electrodes. The Pt counter electrode and the Sb2S3-TiO2 sample were sandwiched and sealed with the conductive sides facing inward. A polysulfide electrolyte was injected into the space between the two electrodes. The polysulfide electrolyte was composed of 0.1 M sulfur, 1 M Na2S, and 0.1 M NaOH which were dissolved in distilled water and stirred at 80°C for 2 h.
A solar simulator (Model 94022A, Newport, OH, USA) with an AM1.5 filter was used to illuminate the working solar cell at light intensity of one sun illumination (100 mW/cm2). A source meter (2400, Keithley Instruments Inc., Cleveland, OH, USA) was used for electrical characterization during the measurements. The measurements were carried out using a calibrated OSI standard silicon solar photodiode.
Results and discussion
Morphology and crystal structure of Sb2S3-TiO2 nanostructure
The morphology of the rutile TiO2 nanorod arrays is shown in Figure 2a. The SEM images clearly show that the entire surface of the FTO glass substrate was uniformly covered with ordered TiO2 nanorods, and the nanorods were tetragonal in shape with square top facets. This nanorod array presented an easily accessed open structure for Sb2S3 deposition and a higher hole transferring speed for the whole solar cell. No significant changes in nanorod array morphology were observed after annealing at 400°C. As-synthesized Sb2S3-TiO2 nanostructure is shown in Figure2b, indicating a combination of the Sb2S3 nanoparticles and TiO2 nanorods. The Sb2S3-TiO2 nanostructure after annealing at 300°C for 30 min is shown in Figure 2c. Compared to the CdS-TiO2 nanostructure, in which 5-to 10-nm CdS nanoparticles distributed uniformly on the TiO2 nanorod , the as-deposited Sb2S3 particles differed with a larger diameter of approximately 50 nm and often covered several TiO2 nanorods. This structural phenomenon was observed much more so in the annealed sample, where at least some melting of the low melting point (550°C) Sb2S3 clearly occurred. After the annealing treatment, the size of Sb2S3 particles increased, which enabled the Sb2S3 particles to closely contact the TiO2 nanorod surface. This solid connection between Sb2S3 nanoparticles and the TiO2 nanorods was beneficial to the charge separation and improved the overall properties of the sensitized solar cells.
X-ray diffraction (XRD) patterns of the bare TiO2 nanorod array, the as-synthesized Sb2S3-TiO2 nanostructure, and the annealed nanostructure are shown in Figure 3. Note in Figure 3a that the TiO2 nanorod arrays grown on the FTO-coated glass substrates had a tetragonal rutile structure (JCPDS no. 02–0494), which may be attributed to the small lattice mismatch between FTO and rutile. The as-synthesized Sb2S3-TiO2 nanostructure exhibited a weak diffraction peak (Figure 3b) at 2θ = 28.7°, corresponding to the (230) plane of orthorhombic Sb2S3. As the annealing temperature increased, more diffraction peaks were observed, and the peaks became more distinct at the same time. Figure 3c shows the XRD pattern of the nanostructure annealed at less than 300°C. All of the reflections were indexed to an orthorhombic phase of Sb2S3 (JCPDS no. c-74-1046) . The shape of the diffraction peaks indicates that the product was well crystallized.
Optical property of the Sb2S3-TiO2 nanostructures
The UV-visible absorption spectra of Sb2S3-TiO2 nanostructure samples are shown in Figure 4. An optical bandgap of 2.25 eV is estimated for the as-synthesized Sb2S3 nanoparticles from the absorption spectra, which exhibits obvious blueshift compared with the value of bulk Sb2S3. After being annealed at 100°C, 200°C, and 300°C for 30 min, the bandgap of Sb2S3 nanoparticles was red shifted to 2.19 eV (565 nm), 2.13 eV (583 nm), and 1.73 eV (716 nm), respectively. When annealed at 400°C, the absorption spectra deteriorated, which may be attributed to the oxidation as well as the evaporation of the Sb2S3 nanoparticles. The Sb2S3-TiO2 nanostructure annealed at 300°C shows an enhanced absorption in the visible range, which is of great importance for solar cell applications and will result in higher power conversion efficiency. As shown by the XRD patterns and SEM images, this red shift in the annealed samples may be explained by the annealing-induced increase in particle size at the elevated temperatures. The annealing effect on the optical absorption spectra of bare TiO2 nanorod arrays was also studied (not included here). No obvious difference was found between the samples with and without annealing treatment. This result suggests that although annealing changes the morphology and crystallinity of Sb2S3 nanoparticles, it does not significantly affect the optical property of TiO2 nanorod arrays.
Photovoltaic performance of the solar cell based on Sb2S3-TiO2 nanostructure
The photocurrent-voltage (I-V) performances of the solar cells assembled using Sb2S3-TiO2 nanostructures annealed under different temperatures are shown in Figure 5. The I-V curves of the samples were measured under one sun illumination (AM1.5, 100 mW/cm2). Compared with the solar cell based on as-grown Sb2S3-TiO2 nanostructure, the solar cell performances correspondingly improved as the annealing temperatures increased from 100°C to 300°C. The open-circuit voltage (Voc) improved from 0.3 up to 0.39 V, and the short-circuit current density (Jsc) improved from 6.2 up to 12.1 mA/cm2. A power conversion efficiency of 1.47% for the sample with annealing treatment was obtained, indicating an increase of 219% (as compared to the 0.46% for the as-grown sample) as a consequence of the annealing treatment. The photovoltaic performance of annealed Sb2S3-TiO2 nanostructured solar cell under 400°C deteriorated, which coincides with the absorption spectrum. Detailed parameters of the solar cells extracted from the I-V characteristics are listed in Table 1.
This significant improvement of the photovoltaic performance obtained for annealed Sb2S3-TiO2 nanostructured solar cells is explained by the following reasons: (1) An enhanced absorption of sunlight caused by the red shift of the bandgap will result in an enhanced current density. (2) Increase of Sb2S3 grain size by annealing will reduce the particle-to-particle hopping of the photo-induced carrier. This hopping may occur in an as-grown nanostructure with Sb2S3 nanoparticles. (3) Improvement of crystal quality of the Sb2S3 nanoparticles by annealing treatment will decrease the internal defects, which can reduce the recombination of photoexcited carriers and result in higher power conversion efficiency. (4) Good contact between the Sb2S3 nanoparticles and the TiO2 nanorod is formed as a result of high-temperature annealing. Such a superior interface between TiO2 and nanoparticles can inhibit the interfacial recombination of the injected electrons from TiO2 to the electrolyte, which is also responsible for its higher efficiency.
Our findings suggest the possible use of 3D nanostructure material grown by a facile hydrothermal method for sensitized solar cell studies. The drawback of this type of solar cell is a rather poor fill factor, which limits the energy conversion efficiency. This low fill factor may be ascribed to the lower hole recovery rate of the polysulfide electrolyte, which leads to a higher probability for charge recombination . To further improve the efficiency of these nanorod array solar cells, we advise that a new hole transport medium with suitable redox potential and low electron recombination at the semiconductor and electrolyte interface should be developed. Moreover, as reported by Soel et al., other contributions such as the counter electrode material may also influence the fill factor .
With a facile hydrothermal method, the single-crystalline TiO2 nanorod arrays were successfully grown on fluorine-doped tin oxide glass. Next, Sb2S3 nanoparticles were deposited by successive ionic layer adsorption and reaction method to form a Sb2S3-TiO2 nanostructure for solar cell applications. Annealing treatment was conducted under varied temperatures, and the optimal annealing temperature of 300°C was obtained. Obvious enhancement in visible light absorption was observed for the annealed samples. The photovoltaic performance for solar cells based on annealed Sb2S3-TiO2 nanostructure shows an increase of up to 219% in power conversion efficiency.
O'Regan B, Grätzel M: A low-cost, high-efficiency solar-cell based on dye-sensitized colloidal TiO2 films. Nature 1991, 353: 737. 10.1038/353737a0
Grätzel M: Photoelectrochemical cells. Nature 2001, 414: 338. 10.1038/35104607
Kao MC, Chen HZ, Young SL, Lin CC, Kung CY: Structure and photovoltaic properties of ZnO nanowire for dye-sensitized solar cells. Nanoscale Res Lett 2012, 7: 260. 10.1186/1556-276X-7-260
Lu LY, Chen JJ, Li LJ, Wang WY: Direct synthesis of vertically aligned ZnO nanowires on FTO substrates using a CVD method and the improvement of photovoltaic performance. Nanoscale Res Lett 2012, 7: 293. 10.1186/1556-276X-7-293
Hossain MF, Zhang ZH, Takahashi T: Novel micro-ring structured ZnO photoelectrode for dye-sensitized solar cell. Nano-Micro Lett 2010, 2: 53.
Yasuo C, Ashraful I, Yuki W, Ryoichi K, Naoki K, HAN LY: Dye-sensitized solar cells with conversion efficiency of 11.1%. Jpn J Appl Phys 2006, 45: 638. 10.1143/JJAP.45.638
Sun WT, Yu Y, Pan HY, Gao XF, Chen Q, Peng LM: CdS quantum dots sensitized TiO2 nanotube-array photoelectrodes. J Am Chem Soc 2008, 130: 1125.
Zhu G, Su FF, Lv T, Pan LK, Sun Z: Au nanoparticles as interfacial layer for CdS quantum dot-sensitized solar cells. Nanoscale Res Lett 2010, 5: 1749. 10.1007/s11671-010-9705-z
Wang CB, Jiang ZF, Wei L, Chen YX, Jiao J, Eastman M, Liu H: Photosensitization of TiO2 nanorods with CdS quantum dots for photovoltaic applications: a wet-chemical approach. Nano Energy 2012, 1: 440. 10.1016/j.nanoen.2012.02.005
Zhang QX, Guo XZ, Huang XM, Huang SQ, Li DM, Luo YH, Shen Q, Toyoda T, Meng QB: Highly efficient CdS/CdSe-sensitized solar cells controlled by the structural properties of compact porous TiO2 photoelectrodes. Phys Chem Chem Phys 2011, 13: 4659. 10.1039/c0cp02099k
Luan CY, Aleksandar V, Andrei SS, Xu XQ, Wang HE, Chen X, Xu J, Zhang WJ, Lee CS, Andrey LR, Juan AZ: Facile solution growth of vertically aligned ZnO nanorods sensitized with aqueous CdS and CdSe quantum dots for photovoltaic applications. Nanoscale Res Lett 2011, 6: 340. 10.1186/1556-276X-6-340
Chen YX, Wei L, Zhang GH, Jiao J: Open structure ZnO/CdSe core/shell nanoneedle arrays for solar cells. Nanoscale Res Lett 2012, 7: 516. 10.1186/1556-276X-7-516
Chen J, Lei W, Deng WQ: Reduced charge recombination in a co-sensitized quantum dot solar cell with two different sizes of CdSe quantum dot. Nanoscale 2011, 3: 674. 10.1039/c0nr00591f
Chen C, Xie Y, Ali G, Yoo SH, Cho SO: Improved conversion efficiency of Ag2S quantum dot-sensitized solar cells based on TiO2 nanotubes with a ZnO recombination barrier layer. Nanoscale Res Lett 2011, 6: 462. 10.1186/1556-276X-6-462
Kieven D, Dittrich T, Belaidi A, Tornow J, Schwarzburg K, Allsop N, Lux-Steiner M: Effect of internal surface area on the performance of ZnO/In2S3/CuSCN solar cells with extremely thin absorber. Appl Phys Lett 2008, 92: 153107. 10.1063/1.2909576
Wang LD, Zhao DX, Su ZS, Shen DZ: Hybrid polymer/ZnO solar cells sensitized by PbS quantum dots. Nanoscale Res Lett 2012, 7: 106. 10.1186/1556-276X-7-106
Maiti N, Im SH, Lim CS, Seok SI: A chemical precursor for depositing Sb2S3 onto mesoporous TiO2 layers in nonaqueous media and its application to solar cells. Dalton Trans 2012, 41: 11569. 10.1039/c2dt31348k
Liu YB, Zhou HB, Li JH, Chen HC, Li D, Zhou BX, Cai WM: Enhanced photoelectrochemical properties of Cu2O-loaded short TiO2 nanotube array electrode prepared by sonoelectrochemical deposition. Nano-Micro Lett 2010, 2: 277.
Wu J, Wang ZM, Dorogan VG, Li SB, Zhou ZH, Li HD, Lee JH, Kim ES, Mazur YI, Salamo GJ: Strain-free ring-shaped nanostructures by droplet epitaxy for photovoltaic application. Appl Phys Lett 2012, 101: 043904. 10.1063/1.4738996
Yafit I, Olivia N, Miles P, Gary H: Sb2S3-sensitized nanoporous TiO2 solar cells. J Phys Chem C 2009, 113: 4254. 10.1021/jp900302b
Moon SJ, Itzhaik Y, Yum JH, Zakeeruddin SM, Hodes G, Gratzel M: Sb2S3-based mesoscopic solar cell using an organic hole conductor. J Phys Chem Lett 2010, 1: 1524. 10.1021/jz100308q
Im SH, Kim HJ, Rhee JH, Lim CS, Seok SI: Performance improvement of Sb2S3-sensitized solar cell by introducing hole buffer layer in cobalt complex electrolyte. Energy Environ Sci 2011, 4: 2799. 10.1039/c0ee00741b
Han QF, Chen L, Zhu WC, Wang MJ, Wang X, Yang XJ, Lu LD: Synthesis of Sb2S3 peanut-shaped superstructures. Mater Lett 2009, 63: 1030. 10.1016/j.matlet.2009.01.078
Lee YL, Chang CH: Efficient polysulfide electrolyte for CdS quantum dot-sensitized solar cells. J Power Sources 2008, 185: 584. 10.1016/j.jpowsour.2008.07.014
Seol M, Ramasamy E, Lee J, Yong K: Highly efficient and durable quantum dot sensitized ZnO nanowire solar cell using noble-metal-free counter electrode. J Phys Chem C 2011, 115: 22018. 10.1021/jp205844r
This work was supported by the National Key Basic Research Program of China (2013CB922303, 2010CB833103), the National Natural Science Foundation of China (60976073, 11274201, 51231007), the 111 Project (B13029), the National Found for Fostering Talents of Basic Science (J1103212), and the Foundation for Outstanding Young Scientist in Shandong Province (BS2010CL036).
The authors declare that they have no competing interests.
YL carried out the preparation of Sb2S3-TiO2 nanostructured solar cells and drafted the manuscript. LW conducted the optical absorption spectra and the I-V measurements. RZ carried out the preparation of TiO2 nanorod arrays and the XRD measurements. YC carried out the SEM characterization and supervised the work. LM and JJ analyzed the results and finalized the manuscript. All authors read and approved the final manuscript.
About this article
Cite this article
Li, Y., Wei, L., Zhang, R. et al. Annealing effect on Sb2S3-TiO2 nanostructures for solar cell applications. Nanoscale Res Lett 8, 89 (2013) doi:10.1186/1556-276X-8-89
- Solar cells
- Annealing effect